Methanol washing effects on spark plasma sintering...
Embed Size (px)
Transcript of Methanol washing effects on spark plasma sintering...
Journal of Ceramic Processing Research. Vol. 8, No. 4, pp. 238~242 (2007)
J O U R N A L O F
Methanol washing effects on spark plasma sintering behavior and mechanicalproperties of B4C ceramics
Kyoung Hun Kim*, Jae Hong Chae, Joo Seok Park, Dae Keun Kima, Kwang Bo Shima and Byung Ha Leeb
Korea Institute of Ceramic Engineering and Technology, Seoul, KoreaaHanyang University, Seoul, KoreabMyongji University, Yongin, Korea
B4C ceramics were fabricated by a spark plasma sintering process and their sintering behavior, microstructure and mechanicalproperties were evaluated. The relative densities of B4C ceramics obtained by spark plasma sintering method reached wereas high as a 99% at lower temperature than used in the conventional sintering method, in addition, without any sinteringadditives. The mechanical properties of B4C ceramics were improved by a methanol washing process which can remove B2O3
coatings from the B4C powder surface. This improvement results from the formation of a fine and homogeneousmicrostructure because the grain coarsening was suppressed by the elimination of the B2O3 coating. In particular, the fracturetoughness of the sintered specimen using a methanol washed powder improved by more than 30% compared with thespecimen using an as-received commercial powder.
Key words: B4C, spark plasma sintering, microstructure, mechanical property.
Boron carbides (B4C) are very useful ceramics in engi-neering applications because of their excellent mechani-cal properties. B4C is a premier material for personalballistic armor because it is the third hardest materialbehind diamond and cubic boron nitride (c-BN), inaddition to its low theoretical density (2.52 g/cm3) .B4C is also used in abrasive applications such as forabrasive powder and nozzles due to its excellentabrasion and wear resistance . Its ability to absorbneutrons without forming long-lived radio nuclides makethe material attractive as an absorbent for the radiationarising in nuclear power plants [1, 2].
It has been reported that the mechanical properties ofB4C ceramics depend on the B/C ratio because boroncarbide exists as a solid solution in the range of 8.8 to20 at% carbon (B10.5C-B4C) [3-5]. Niihara et al. report-ed that the hardness and fracture toughness values weremaximum at essentially the stoichiometric compositionB/C = 4 and decreased for B/C<4 (composition regionof B4C + C) and for B/C > 4 (non-stoichio-metric regionof B4C) .
Effective ballistic armor should have a very highhardness combined with a high fracture toughness [6, 7].In general, these mechanical properties are closelyrelated to chemical com-position and microstructure.
Densification of pure B4C is quite difficult because of itsstrong covalent bonding characteristics. Although, highdensity pure B4C ceramics which have up to 95% rela-tive density may be obtained using a hot-press sinteringmethod at least at 2200 oC, deterioration of mechanicalproperty was inevitable because of microstructural coar-sening at a high sintering temperature [8-10].
Additives such as SiC, TiB2, Al2O3 and some transi-tion metals have been used as sintering aids to fabricateB4C ceramics [11-14]. The best known sintering additivefor B4C is carbon, commonly added in the form ofphenol resin, which can remove the boron oxide phasefrom the powder surface and induce a non-stoichiometriccomposition during the sintering process, consequentlyaccelerating densification via enhanced grain boundarydiffusivity [6, 10, 15, 16]. However, the non-stoichiometricboron carbide composition and the secondary phasesinduced by the additives often have deleterious effectson the mechanical properties [1, 5].
Recently, the spark plasma sintering (SPS) processhas gained significant interest for fabrication of poorlysinterable materials such as borides, carbides and nitrides.The SPS process is a type of pressure sintering methodwhich uses a high-temperature spark plasma generatedby discharging the gaps between powder particles withon-off electrical current . The generation of thespark plasma in the initial stage of the SPS processaccelerates the neck formation and thermal diffusion,and has a surface-activating and cleaning effect on theparticles being sintered. Also, the electrical field form-ed by the DC current accelerates diffusion. Therefore,the SPS process has been applied for densification of
*Corresponding author: Tel : +82-2-3282-7870Fax: +82-2-3282-2490E-mail: [email protected]
Methanol washing effects on spark plasma sintering behavior and mechanical properties of B4C ceramics 239
poorly sinterable materials at lower temperatures and inshorter times than is impossible with conventionalsintering process [17-19].
The present study is an attempt to use SPS to obtainfully densified B4C ceramics without additives in orderto improve in the mechanical properties. In particular,we have studied the effect of methanol washing of B4Cpowder which can remove boron oxide (B2O3) coatingsfrom the particle surfaces . The presence of B2O3
coatings on B4C particles inhibits densification untilthey are volatilized away, and this facilitates B4C parti-cle coarsening resulting in microstructural coarsening[10, 21].
Commercially available B4C powder (HS grade, H.C.Starck, Germany) was used as a starting material. Table1 shows the characteristics of the powder based on themanufacture’s data. The commercial B4C powder wassuspended in methanol (99.9%, J.T. Baker, USA) andultrasonicated (B3200, Branson, USA) for 1 hour. Thesuspension was then placed in a dry oven at 80 oC for12 hours to volatilize the methanol. This process wasrepeated three times for the purpose of removing B2O3
coatings from the surfaces .The powders were loaded into a graphite mold inside
the SPS system (Dr. Sinter 515S, Sumitomo Coal andMining Co., Japan). After applying an initial pressureof 40 MPa, the loaded powers were heated in thesintering temperature range from 1800 oC to 2000 oCfor 5 minutes at a heating rate of 100 K/minute in avacuum (<10 Pa). After finishing the sintering process,the pressure was relaxed and the specimens were cool-ed in the chamber. The sintered bodies were typically15 mm in diameter and 4 mm in thickness.
The density was measured by the Archimedes methodand an X-ray diffractometer (M03XHF22, MAC ScienceCo., Japan) was used for analyzing the phases in thepowders and sintered bodies. The hardness and fracturetoughness were measured using a Vickers indenter (HM-
124, Akashi, Japan) with a 9.8 N load for 15 seconds.The microstructural charac-terization was carried outwith scanning electron microscope (SEM, 5900LV, JEOL,Japan) after electrolytic etching in 1% KOH solutionfor 30 seconds with 3.5 V and 0.1 A/cm2. The averagegrain size was calculated using the linear intercept method(ASTM E 112-96) based on 1000 measurements onSEM micrographs.
Results and Discussion
Figure 1 shows XRD patterns of the B4C powdersand sintered bodies at 2000 oC. B2O3 peaks weredetected in the commercial powder, but they wereremoved from the methanol washed powder. This resultindicates that the methanol washing process is veryeffective in removing B2O3 coatings from the B4Cpowder surfaces. Also, B2O3 peaks were removed fromthe sintered body using a commercial powder becausethe B2O3 phase has a tendency to vaporize above1200 oC [6, 10].
Figure 2 shows the relative density of specimens as afunction of sintering temperature. The final density ofeach powder was not affected by the conditions of their
Table 1. Characteristics of B4C powder
Specific surface area =<18 m2/g
Particle sizeD 90% of particles 3.0 μmD 50% of particles 0.8 μmD 10% of particles 0.2 μm
Max. 1.70 wt% of OMax. 0.70 wt% of NMax. 0.05 wt% of FeMax. 0.15 wt% of SiMax. 0.05 wt% of AlMax. 0.50 wt% of other
Total boronTotal carbonB/C molar ratio
75.65 wt%21.2 wt%03.7
Fig. 1. XRD patterns of commercial B4C powder, methanolwashed powder and sintered bodies at 2000oC.
Fig. 2. Variation of relative density of commercial and methanolwashed specimens as a function of sintering temperature.
240 Kyoung Hun Kim, Jae Hong Chae, Joo Seok Park, Dae Keun Kim, Kwang Bo Shim and Byung Ha Lee
surfaces but depended on the sintering temperature.The relative density dramatically increased at 1850 oCup to 95%, and it reached over 99% at 1900 oC. It isvery difficult to obtain full density pure B4C ceramicsat such a low temperature, 1900 oC, using conventionalsintering methods. This result demonstrated the excel-lent sinterability of the SPS process.
Figure 3 shows the displacement of the total heightof the graphite mold assembly during the SPS processat 1950 oC. This displacement directly represents theshrinkage profile during densification of the powders inreal time. It is seen that the commercial B4C powder
starts to densify at about 1620 oC, but the methanolwashed powder begins at about 1530 oC. The resultclearly shows that the presence of B2O3 coatings on thesurfaces of B4C particles delayed the onset of sintering.The removal of B2O3 coatings permitted direct B4C-B4C contact resulted in low temperature densificationby the acceleration of lattice and / or grain boundarydiffusion [6, 8, 15].
Figure 4 shows the change in average grain size withthe sintering temperature. The average grain size of thecommercial powder specimens was larger than that of
Fig. 4. The change of average grain sizes of commercial andmethanol washed specimens as a function of sintering temperature.
Fig. 5. SEM micrographs of etched surface B4C specimens sintered at (a) 1850 oC, (b) 1900 oC, (c) 1950 oC and (d) 2000 oC usingcommercial powder.
Fig. 3. Densification behavior of B4C powders during the sparkplasma sintering process.
Methanol washing effects on spark plasma sintering behavior and mechanical properties of B4C ceramics 241
methanol washed powder specimens. In general, the graincoarsening of covalently bonded materials originatesfrom surface diffusion and an evaporation-condensationmechanism. It has been suggested that the existence ofB2O3 coatings may provide a rapid diffusion path onparticle surfaces because the firing temperatures arewell above its melting point, 450 oC . Also, thevolatility of B2O3 causes the microstructural coarseningabove 1500 oC because the vapor pressure of B2O3 issufficiently high for mass transport . Thus theretardation of densification (as indicated in Fig. 3) andthe microstructural coarsening are due to the existenceof B2O3 phases on the particle surfaces.
Figure 5 and Fig. 6 show the etched surface morpho-logy of sintered bodies at different sintering temper-atures using the commercial B4C powder and the meth-anol washed B4C powder, respectively. A near fullydense microstructures are shown in both specimensabove 1950 oC. The grain coarsening during SPS sinter-ing is clearly seen in the commercial powder specimen(as shown in Fig. 5) with increase sintering temper-ature. However, the microstructure of methanol washedspecimens (as shown in Fig. 6) is finer and morehomogeneous than that of commercial powder speci-mens. Referring to the result of average grain sizeshown in Fig. 4, these results show that the removal ofB2O3 coatings is very effective in restricting the graincoarsening and consequently in obtaining a fine and
homogeneous microstructure.Figure 7 and Fig. 8 show Vickers hardness and
fracture toughness, respectively, of sintered bodies as afunction of sintering temperature using the commercialB4C powder and the methanol washed B4C powder.The increase of Vickers hardness values (as shown inFig. 7) of both samples with increase sintering temper-ature up to 1950 oC may have originated from theincrease of density and the values are saturated above1950 oC. The Vickers hardness value of methanol wash-ed specimens is higher than that of commercial specimensbecause the methanol washed specimens have a smaller
Fig. 6. SEM micrographs of etched surface B4C specimens sintered at (a) 1850oC, (b) 1900 oC, (c) 1950 oC and (d) 2000 oC using methanolwashed powder.
Fig. 7. Variation of Vickers hardness of commercial and meth-anol washed specimens as a function of sintering temperature.
242 Kyoung Hun Kim, Jae Hong Chae, Joo Seok Park, Dae Keun Kim, Kwang Bo Shim and Byung Ha Lee
grain size. In particular, the improvement in the fracturetoughness (as shown in Fig. 8) is significant for themethanol washed B4C powder. The fracture toughnessof methanol washed specimens increased by more than30% over the commercial specimens. The fine andhomogeneous micro-structure make a great contribu-tion to the improvement of the mechanical properties.
Poorly sinterable B4C ceramics were successfully fullydensified even without additives at a lower temperaturethan by using a conventional sintering method. Themicrostructural coarsening was effectively inhibited bythe removal of boron oxide coatings on B4C particlesurfaces by the methanol washing process. The removalof B2O3 coatings could permit a direct B4C-B4C contactwhich resulted in low temperature densification andsuppression of coarsening by the acceleration of latticeand / or grain boundary diffusion. As a result, themechanical properties were significantly improved by
the formation of a fine and homogeneous microstruc-ture.
1. F. Thevenot, J. Euro. Ceram. Soc. 6 (1990) 205-225.2. D. Simeone, C. Mallet, P. Dubuisson, G. Baldinozzi, C.
Gervais, and J. Maquet, J. Nucl. Mater. 277 (2000) 1-10.3. J. Beauvy, J. Less Common Metals 90 (1983) 169-175. 4. R.D. Allen, J. Am. Chem. Soc. 75 (1953) 3582-3583. 5. K. Niihara, A. Nakahira, and T. Hirai, J. Am. Ceram. Soc.
67 (1984) c13-c14. 6. H. Lee and R.F. Speyer, J. Am. Ceram. Soc. 86 (2003)
1468-1473.7. M. Grujicic, B. Pandurangan, K.L. Koudela, and B.A.
Cheeseman, App. Surf. Sci. 253 (2006) 730-745. 8. R.M. Spriggs and S.K. Dutta, in “Sintering and Related
Phenomena” (Plenum Press, 1973) p. 369-3949. R. Angers and M. Beauvy, Ceram. Int. 10 (1984) 49-55.
10. S.L. Dole, S. Prochazka, and R.H. Doremus, J. Am. Ceram.Soc. 72 (1989) 958-966.
11. T. Vasilos, and S.K. Dutta, Am. Ceram. Soc. Bull. 53(1974) 453-454.
12. Y. Kanno, K. Kawase, and K. Nakano, J. Ceram. Soc. Jpn.95 (1987) 1137-1140.
13. V. Skorokhod Jr., M.D. Vlajic, and V.D. krstic, J. Mater.Sci. Lett. 15 (1996) 1337-1339.
14. C.H. Lee and C.H. Kim, J. Mater. Sci. 27 (1992) 6335-6340.
15. C. Greskovich, and J.H. Rosolowski, J. Am. Ceram. Soc.59[7/8] (1976) 336-343.
16. K. Schwetz and G. Vogt, US Patent 4,195,066 (1980).17. M. Tokita, J. Soc. Powder Tech. Jpn. 30 (1993) 790-
804.18. M. Omori, Mater. Sci. Eng. A 287 (2000) 183-188.19. K.H. Kim and K.B. Shim, Mater. Character. 50 (2003) 31-
37.20. P.D. Williams and D.D. Hawn, J. Am. Ceram. Soc. 74
(1991) 1614-1618.21. H. Lee, W.S. hackenberger, and R.F. Speyer, J. Am.
Ceram. Soc. 85 (2002) 2131-2133.
Fig. 8. Variation of fracture toughness of commercial and meth-anol washed specimens as a function of sintering temperature.